Biomaterials 50 (2015) 38e46
Contents lists available at ScienceDirect
Biomaterials journal homepage: www.elsevier.com/locate/biomaterials
Towards long lasting zirconia-based composites for dental implants. Part I: Innovative synthesis, microstructural characterization and in vitro stability Paola Palmero a, *, Marta Fornabaio a, Laura Montanaro a, Helen Reveron b, ro ^ me Chevalier b, c Claude Esnouf b, Je a b c
Department of Applied Science and Technology, INSTM R.U. PoliTO, LINCE Lab., Politecnico di Torino, Corso Duca degli Abruzzi, 24, 10129 Torino, Italy Universit e de Lyon, INSA de Lyon, MATEIS CNRS UMR5510, 20 Avenue Albert Einstein, F-69621 Villeurbanne Cedex, France Institut Universitaire de France, 103 bd Saint-Michel, Paris 75005, France
a r t i c l e i n f o
a b s t r a c t
Article history: Received 12 September 2014 Accepted 20 January 2015 Available online
In order to fulﬁll the clinical requirements for strong, tough and stable ceramics used in dental applications, we designed and developed innovative zirconia-based composites, in which equiaxial a-Al2O3 and elongated SrAl12O19 phases are dispersed in a ceria-stabilized zirconia matrix. The composite powders were prepared by an innovative surface coating route, in which commercial zirconia powders were coated by inorganic precursors of the second phases, which crystallize on the zirconia particles surface under proper thermal treatment. Samples containing four different ceria contents (in the range 10.0e11.5 mol%) were prepared by carefully tailoring the amount of the cerium precursor during the elaboration process. Slip cast green bodies were sintered at 1450 C for 1 h, leading to fully dense materials. Characterization of composites by SEM and TEM analyses showed highly homogeneous microstructures with an even distribution of both equiaxial and elongated-shape grains inside a very ﬁne zirconia matrix. Ce content plays a major role on aging kinetics, and should be carefully controlled: sample with 10 mol % of ceria were transformable, whereas above 10.5 mol% there is negligible or no transformation during autoclave treatment. Thus, in this paper we show the potential of the innovative surface coating route, which allows a perfect tailoring of the microstructural, morphological and compositional features of the composites; moreover, its processing costs and environmental impacts are limited, which is beneﬁcial for further scale-up and real use in the biomedical ﬁeld. © 2015 Elsevier Ltd. All rights reserved.
Keywords: Zirconia Alumina Composite Microstructure Ageing Dental implant
1. Introduction The excellent mechanical properties of zirconia-based materials combined with their superior aesthetics and biocompatibility characteristics have enlarged, in the last years, their application in the dental ﬁeld. Particularly, the high strength (>1200 MPa)  exhibited by yttria-stabilized zirconia ceramics (Y-TZP) allows them withstanding intermittent forces that arise throughout mastication, thus becoming very interesting materials in prosthetic
* Corresponding author. DISAT, Politecnico di Torino, Corso Duca degli Abruzzi, 24, 10129 Torino, Italy. Tel.: þ39 011 0904678; fax: þ39 011 0904624. E-mail address: [email protected]
(P. Palmero). http://dx.doi.org/10.1016/j.biomaterials.2015.01.018 0142-9612/© 2015 Elsevier Ltd. All rights reserved.
dentistry. Nowadays, fully dense, translucent yttria-stabilized zirconia ceramics can be processed with ﬁne grains size (0.3 mm), thus meeting esthetic and mechanical requirements . However, the tetragonal (t) to monoclinic (m) transformation speciﬁc of (meta) stabilized zirconia, which is responsible of these extraordinary properties, can also induce a negative phenomenon known as Low Temperature Degradation (LTD), or aging . It consists in a slow transformation of t-zirconia to the m phase (without any applied stress) in a wide temperature range, typically from room temperature up to around 400 C, thus including the temperature used for steam sterilization (~140 C) and the human body temperature (37 C) [4,5]. Possible consequences are loss of strength and generation of micro-cracks .
P. Palmero et al. / Biomaterials 50 (2015) 38e46
This phenomenon has been well investigated by the orthopedic community since 2001, when a large series of failures of Y-TZP femoral heads was reported . Although the manufacturing process of orthopedic zirconia femoral heads is signiﬁcantly different from that of dental zirconia, some studies have recently focused on LTD in the dental ﬁeld [8e13]. Cattani-Lorente et al.  and Kohorst et al.  observed the reduction of mechanical properties of Y-TZP dental ceramics after LTD. Chevalier et al.  evaluated novel porous zirconia dental implants and reported their aging sensitivity. Kim et al.  described the inﬂuence of different surface treatments on LTD behavior of dental zirconia. Finally, Denry et al.  reported that some forms of zirconia are susceptible to aging and that processing conditions can play a critical role in the LTD behavior. Therefore, as well as for orthopedic applications, current research is now focusing on alternative zirconia-based materials to Y-TZP, especially for implants for which the translucency is less important but for which a perfect stability at long durations must be insured in contact with body ﬂuid. Beside the composites in the alumina-zirconia systems [14e17], ceria-stabilized zirconia (CeTZP) seems a promising candidate due to its reduced susceptibility to aging and its excellent fracture toughness [18,19]. However, these attractive properties of Ce-TZP are countervailed by its low strength (about 500 MPa ) that still prevents its use in biomedical applications. Hence, it is essential to move to composite systems in which the presence of a well-distributed second phase is widely recognized to enhance mechanical properties. Fracture toughness of about 9.8 MPa√m and a mean strength of 950 MPa was reported by Nawa et al. [20,21] for Ce-TZP-based composites containing 30 vol% of Al2O3. Higher fracture toughness (about 15 MPa√m) and comparable strength (900 MPa) were recently reported by Apel et al. for 10Ce-TZP/MgAl2O4 composite . Both these systems, characterized by an inter/intra-granular nano-structure, highlight the necessity to carefully tailor and reﬁne the microstructure in order to fulﬁll the requirements for biomedical ceramics. Since the microstructure is signiﬁcantly affected by the process conditions (such as powder synthesis and sintering), a deeper understanding of the relationship between microstructure and processing is a key issue to predict mechanical properties. Among the several elaboration techniques to process zirconiabased composite powders, the most common are the traditional powder milling and mixing method and the co-precipitation route [23e25]. The former, a simple and fast procedure, often yields to materials with severe limitations for what concerns the ﬁnal phase purity and microstructural homogeneity. On the other hand, coprecipitation route makes it possible to overcome such limitations, but implies expensive chemical precursors and the whole process is much more complex to manage. Recently, a novel processing route has been developed to produce composite powders via surface coating technique [26e28]. Starting from a commercial powder, its surface is coated (or graft) by precursors of the second phase, which crystallizes on the surface of the parent material under proper thermal treatment. The close mixing between the matrix ceramic particles and the precursor is realized at nano/ atomic level, assuring an excellent distribution of the second phase in the composite material . In this context, the European project named LongLife “Advanced multi-functional zirconia ceramics for long-lasting implants” (7th Framework Program) aims at developing new multi-functional zirconia-based ceramics having a perfect reliability and a lifetime longer than 60 years. To reach this goal, efforts should focus on the improvement of the zirconia stability in the presence of water, while maintaining high toughness and strength. In this paper the strategy of LongLife towards strong, tough and stable zirconiabased materials is presented implying i) the design of innovative ultra-ﬁne composite structures and ii) the use of a new approach
named nano-powder engineering. Such approach allows a perfect tailoring of the compositional and microstructural features in the developed materials. This is the objective of the Part I of the work, aimed at developing materials designed for dental applications. A comprehensive set of mechanical properties of the developed materials in terms of Vickers hardness, ﬂexural strength and fracture toughness will be reported in Part II, ﬁnally showing the potential use of these composites as dental ceramics. Concerning the composite design, we chose Ce-TZP as composite matrix, due to its reduced susceptibility to aging as respect to Y-TZP, and two kinds of second phases characterized by different morphologies: equiaxed and elongated. The role of well-dispersed, ﬁne equiaxed particles is to reﬁne the Ce-TZP microstructure by a pinning effect exerted on the zirconia grain boundaries during the sintering cycle. Although reﬁning microstructure increases strength, hardness and wear resistance [29,30], it inevitably decreases the efﬁciency of the phase transformation toughening . In order to obtain high transformability under stress even with very ﬁne-grained structures, in the present study the ceria content in the composite materials is carefully tailored. In addition, the formation of elongated second-phase particles is promoted, with the aim of further increasing the toughness by additional bridging/crackdeﬂection mechanisms [32,33]. Precisely, on the ground of the previous scientiﬁc literature [15,32e35] a-Al2O3 and strontium hexa-aluminate, SrAl12O19, were selected as second-phases and added to the Ce-TZP matrix. A preliminary investigation on the biocompatibility of this composite powder showed already promising results in terms of bacterial adhesion, as reported by Karygianni et al. , further supporting its employment in the biomedical ﬁeld. Fig. 1 shows a schematic strength-toughness relationship for many Y-TZP and Ce-TZP-based materials, according to literature data [1,19e22,30,32,33,37]. It is striking the lack of materials able to meet all the requirements for dental implants (i.e. perfect stability in vivo, very high strength and fracture toughness) thus clarifying the objective of LongLife, depicted in the same Figure. The “Longlife composites” are not a new family of zirconia based composites since some studies on (almost) similar compositions are already present in literature [32,34]. However, the innovation and objective of this work is the development of such composites through an innovative surface coating method, simple but very effective in assuring a perfect control of all the microstructural and compositional features of the composite structures. Other surface-
Fig. 1. Relationship strength-toughness for several zirconia-based materials. In green, the objective of LongLife towards LTD-free, strong and tough composites.
P. Palmero et al. / Biomaterials 50 (2015) 38e46
coating methods were previously reported in literature by Schehl et al.  and Yuan et al. , but all using organic media to process the composite powders. On the opposite, our method developed in the last years for alumina-based composites  and applied in this study e for the ﬁrst time e to zirconia-based multi-phase composites, implies the use of only inorganic precursors and aqueous media. In this way, processing costs and environmental impacts of the surface-coating methods can be limited. The process, recently described in an Italian Patent application (TO2014A000145), seems well qualiﬁed to be employed, after proper scaling-up, in the industrial manufacturing processes. 2. Materials and methods 2.1. Elaboration of the composite powder A commercial 10 mol% ceria-stabilized zirconia powder (supplied by Daiichi Kigenso Kagaku Kogio Co. LTD, Japan, referred to as 10Ce-TZP) was employed as raw material to develop composite powders having the following composition: 84 vol% ZrO2 e 8 vol% Al2O3 e 8 vol% SrAl12O19 (referred to as ZA8Sr8). The starting 10Ce-TZP powder is characterized by a speciﬁc surface area of 14.3 m2/g and an average particle size (by laser diffraction method) of 0.5e1 mm . Al(NO3)3$9H2O (>98% purity, SigmaeAldrich) and Sr(NO3)2 (>99.0% purity, SigmaeAldrich) were used as aluminum and strontium precursors, respectively. In order to modify and tailor the ceria content in the powders, ammonium cerium nitrate ((NH4)2[Ce(NO3)6], 98.5% purity, SigmaeAldrich) was used as cerium precursor. First, the zirconia powder was dispersed in distilled water at a solid loading of 8 vol% by ball milling for about 15 h. A pH of 3 was reached by adding diluted hydrochloric acid and this value was maintained all over the process. Zirconia spheres (2.0 mm in diamater, Tosoh Corporation) were selected as milling media since they exhibit high crushing strength and wear resistance . They were used in a weight ratio of 1:10 with respect to the powder. In order to avoid product contamination, zirconia grinding media were periodically replaced. The particle size distribution was determined by using laser-granulometry (Fristch Analysette 22). The nitrates were then dissolved in distilled water, until clear solutions were obtained. Zirconia to aluminum nitrate weight ratio of 1:0.838 and zirconia to strontium nitrate weight ratio of 1:0.018 were used. In addition, zirconia to cerium nitrate weight ratios of 1:0.02, 1:0.04 and 1:0.06 were employed to obtain 10.5, 11.0 and 11.5 mol%, respectively, of ceria in the zirconia phase. The cerium salt concentration was determined by considering a CeO2 amount of 10 mol% already present in the raw zirconia powder, as declared by the supplier, and assuming its complete diffusion inside the zirconia lattice during thermal treatments . The nitrate solutions were drop-wise added to the dispersed zirconia slurry; the modiﬁed suspension was kept under magnetic stirring for 2 h to assure homogeneity and ﬁnally spray-dried. In order to clarify the ceria molar content in the ﬁnal composites, powders are referred to as ZA8Sr8-Ce10, ZA8Sr8-Ce10.5, ZA8Sr8-Ce11 and ZA8Sr8-Ce11.5, being the former composite the only one in which no extra-cerium was added during synthesis. The as-spray dried powders were submitted to Thermogravimetric and Differential Thermal Analyses (TG-DTA, Netzsch STA 409C) carried out up to 1400 C (heating and cooling rate of 10 C/min, under static air). On the basis of TG-DTA curves, the doped powders were pre-treated at 600 C for 1 h at the heating rate of 10 C/min with the aim of inducing the decomposition of the by-products. In addition, a second pre-treatment was carried out in the 900e1450 C temperature range to induce the crystallization of the second phases on the zirconia particle surface. The crystalline phases were analyzed by XRD diffraction (Philips PW 1710) with a Cu Ka anticathode in the 10e70 range in 2 theta (a step size of 0.05 and a time for step of 5 s).
2.2. Forming and sintering Green bodies were prepared by slip casting, which requires the preparation of stable suspensions with suitable solid loading. For this reason, aqueous suspensions of the pre-treated composite powders at a solid loading of 26 vol% were prepared and dispersed by ball-milling for about 30 h. In order to increase the powder dispersibility and to yield stable suspensions, 3 wt% (as respect to the powder weight) of a commercial dispersant (Duramax D-3005) was added. The evolution of the particle size distribution within the dispersion time was determined by lasergranulometry. Green bodies were obtained by casting the dispersed slurries into pure alumina porous molds followed by a drying step into a humidity-controlled chamber for about 1 week. Debinding was carried at 600 C for 1 h (heating and cooling rate of 5 C/min). The densiﬁcation behavior was investigated by dilatometric analyses (Netzsch 402E) by heating up to 1500 C, for 1 h. Tests were carried out at three different heating rates, being precisely 2, 5 and 10 C/min.
Materials were obtained by pressureless sintering in the temperature range 1400e1450 C, for different dwell times (1e2 h). As a comparison, 10Ce-TZP and 3YTZP reference materials were also prepared. Slip cast 10Ce-TZP was sintered in the 1450 Ce1500 C for 1e3 h, whereas granules of 3Y-TZP were cold isostatic pressed and sintered at 1450 C for 2 h, following the standard procedure reported in literature for this material . 2.3. Characterizations The green and ﬁred densities were evaluated by mass-geometric measurements and Archimedes method and referred to the materials theoretical density (TD), calculated by the rule of mixtures for composite systems (values of 6.19, 5.82, 3.99 and 4.02 g/cm3 for tetragonal and monoclinic ZrO2, a-Al2O3 and SrAl12O19 were respectively used). The phase composition was investigated by XRD, and the monoclinic volume content (Vm) was determined by applying the Toraya's equation . The microstructures were analyzed by means of Scanning Electron Microscopy (SEM Zeiss SUPRA VP55) and Field Emission Scanning Electron Microscopy (FESEM Hitachi S4000) on polished and thermally etched specimens. The mean grain sizes of matrix and second phases were determined by image analysis (Scandium Soft imaging system software). In addition, high-resolution Transmission Electron Microscopy (HRTEM JOEL 2010 F) equipped for EDX nanoprobe analyses and X-rays mapping was used on selected composition (ZA8Sr8-Ce11). Selected Area Diffraction (SAED) and Fast Fourier Transform (FFT) of the HRTEM images from DigitalMicrograph™ software were used to index the crystalline phases. Finally, the sintered materials were submitted to preliminary hydrothermal aging tests, with the aim of investigating the role of the ceria content on the in-vitro stability. The tests were performed in autoclave (Fisher Bioblock Scientiﬁc) at 134 C under 2 bar pressure. After controlled period of time, XRD analysis was carried out in order to evaluate the content of the monoclinic phase during the aging test.
3. Results and discussion 3.1. Elaboration of the composite powders Ball milling was effective in dispersing the starting zirconia agglomerates to the desired particle size: the mean diameter of the volume distribution (d50) decreased from 1.1 to 0.5 mm as reported in Table 1. In Fig. 2, a SEM micrograph of the dispersed powder is depicted, showing a small agglomerate, of about 0.5 mm, in which primary particles of less than 100 nm can be easily recognized. Nitrates aqueous solutions were added to such dispersed powder and the suspension was spray dried. This is a key point of the process since a ﬁne dispersion of the raw powder and a fast drying step assure a homogeneous coating of zirconia particles by the precursors of the second-phases. As a consequence, a homogeneous distribution of the second phases in the ﬁnal composite materials can be achieved . In order to avoid aluminum hydroxide precipitation , the pH of the suspension was kept stable at a value of 3. In Fig. 3 the TG-DTA curves of the spray-dried ZA8Sr8-Ce11 powder are depicted. The TG curve shows a mass loss of about 30%, due to the decomposition of the synthesis byproducts (mainly the nitrates), which was almost accomplished at about 500 C. Accordingly, after spray drying, all powders were calcined at 600 C for 1 h, in order to assure the precursors decomposition. The DTA curve shows a broad, exothermic peak at about 1200 C, imputable to both a-Al2O3 and SrAl12O19 crystallization. Precisely, as reported by Douy et al. , it is supposed that alumina crystallizes into the g-Al2O3 phase at about 950 C,
Table 1 Diameters (d10, d50 and d90) of the particle size distribution before and after ballmilling (BM) of 10Ce-TZP and ZA8Sr8-Ce11 powder.
10Ce-TZP before BM 10Ce-TZP after BM ZA8Sr8-Ce11 before BM ZA8Sr8-Ce11 after BM a
0.5 n.d.a 11 n.d.a
1.1 0.5 42 0.5
2.3 0.8 255 0.9
n.d. means below the instrumental limit (